- Research article
- Open Access
Modification and optimization of electrospun gelatin sheets by electron beam irradiation for soft tissue engineering
© The Author(s). 2017
- Received: 26 May 2017
- Accepted: 22 June 2017
- Published: 11 July 2017
Crosslinked gelatin nanofibers are one of the widely used scaffolds for soft tissue engineering. However, modifying the biodegradation rate of chemically crosslinked gelatin is necessary to facilitate cell migration and tissue regeneration. Here, we investigated the optimal electron beam (e-beam) irradiation doses with biodegradation behavior on changes in the molecular weight, morphology, pore structure, and cell proliferation profiles of electrospun nanofibrous gelatin sheets.
The molecular weights of uncrosslinked gelatin nanofibers were measured using gel permeation chromatography. The morphology and pore structure of the gelatin scaffolds were analyzed by scanning electron microscopy and a porosimeter. Biodegradation tests were performed in phosphate-buffered saline solutions for 4 weeks. Cell proliferation and tissue regeneration profiles were examined in fibroblasts using WST-1 assays and hematoxylin and eosin staining.
Crosslinked gelatin nanofiber sheets exposed to e-beam irradiation over 300 kGy showed approximately 50% weight loss in 2 weeks. Gelatin scaffolds exposed to e-beam irradiation at 100–200 kGy showed significantly increased cell proliferation after 7 days of incubation.
These findings suggested that the biodegradation and cell proliferation rates of gelatin nanofiber scaffolds could be optimized by varying e-beam irradiation doses for soft tissue engineering.
- Electron beam
Gelatin, a protein derived from controlled hydrolysis of collagen, is potentially useful as a biomaterial because of its biological origin, biocompatibility, non-antigenicity, and biodegradability. Furthermore, the existence of unique sequences of amino acids and many functional side groups makes it easy to modulate its physicochemical properties [1–3]; thus, gelatin has been widely used as tissue engineering scaffold, drug delivery carrier, wound dressing, and sealant for vascular prostheses in the biomedical field. However, gelatin must be modified for use in biomedical applications because it is soluble in aqueous solution and shows mechanical weakness. The typical technique for gelatin modification is crosslinking with a variety of chemical and physical treatments [1, 4–8]. Researchers have studied various crosslinking methods, including chemical crosslinking with glutaraldehyde, 1-ethyl-3-(3-dimethylamino propyl) carbodiimide hydrochloride (EDC), and genipin and physical crosslinking (e.g., dehydrothermal treatment or exposure to plasma, UV, and γ-radiation). Generally, chemical methods have high efficiency for stabilization of crosslinked gelatin; however, the degree of transformation cannot be controlled precisely [9, 10]. Furthermore, highly crosslinked gelatin materials are not suitable for use in vitro because they are rarely hydrolyzed without enzyme. In contrast, physical methods provide cost-efficient and environmentally friendly alternatives, but yield a lower degree of crosslinking. Mediation of the crosslinking type for gelatin is necessary to achieve desirable properties for particular biomedical applications.
Among reported physical crosslinking methods, ionizing irradiation treatment with γ-ray or electron beam (e-beam) radiation is operationally fast and does not require additives or severe conditions, which could deform the material structure [11–20]. Moreover, the high energy of irradiation can cause both crosslinking and degradation of the material and alter the physical and chemical characteristics of the material through main chain scission and crosslinking. After irradiation, excited polymers, such as reactive intermediates, ions, and free radicals, are formed, and these active species create new bonds and alter material properties as a result of initiation or free reaction among the polymer chain [16, 21, 22]. Crosslinking occurs when two radicals induced by irradiation combine to form a covalent bond, leading to an increase in molecular weight. In contrast, degradation arises out of high energy in excess of the attractive forces between atoms, thus rupturing the chemical bonds and causing a decrease in molecular weight. As a result of these reactions, ionizing radiation is related to the lifespan of the materials via crosslinking and chain scission.
Although some studies have assessed the effects of γ-radiation on gelatin, very few studies have investigated the effects of e-beam irradiation on gelatin [12–17]. Accordingly, in this study, we focused on the effects of e-beam irradiation on changes in the molecular weight, morphology, and biodegradation rate of nanofibrous gelatin sheet scaffolds. The primary objective of this study is to assess the e-beam irradiation dosage on gelatin nanofiber sheets in order to optimize the biodegradation rate for use as a soft tissue engineering scaffold.
Electrospinning of gelatin nanofibers
Type B gelatin (250 bloom) was obtained from Geltech Co., Korea, and 2,2,2-trifluoroethanol (TFE) was purchased from Sigma-Aldrich (USA). Gelatin nanofiber sheets were fabricated using electrospinning of a gelatin-TFE solution. Gelatin was dissolved in TFE at 10% (w/v) by stirring overnight at room temperature. Electrospinning was performed using a 10-mL polypropylene syringe with a 21-gauge needle. A high voltage of 15 kV was applied to the needle and stainless steel drum collector (drum diameter: 23 cm). The distance between the needle and collector was set as 12 cm. The flow rate of the gelatin-TFE solution was 2 mL/h. The electrospun sheets were placed in a vacuum oven overnight at room temperature to remove a residual solvent.
Crosslinking of nanofibrous gelatin sheets
Gelatin nanofiber sheets were crosslinked by glutaraldehyde (25%; Daejung Chemicals & Materials Co., Ltd., Korea). The vapor crosslinking process was carried out for 6 h in a sealed desiccator with 25% glutaraldehyde (10 mL) in a petri dish [5, 6]. Electrospun gelatin sheets were placed on a stainless steel wire net in the desiccator to avoid uneven crosslinking and crosslinked with the glutaraldehyde vapor at 25 °C. After crosslinking, the samples were placed in a vacuum oven for 24 h to prevent excessive crosslinking by removing residual glutaraldehyde. Crosslinked gelatin nanofiber sheets were kept at 4 °C before use.
E-beam irradiation of the gelatin nanofibrous sheets was performed using an Electron Beam Accelerator (ELV-8; EB Tech Co., Ltd., Korea). Uncrosslinked and crosslinked gelatin samples were irradiated to investigate the effects of e-beam radiation. For uncrosslinked gelatin, irradiation of the e-beam was carried out in an air and N2 atmosphere at room temperature. The irradiation doses were 10, 20, 30, 40, 50, 60, 70, 80, 90, 100, 150, 200, 250, and 300 kGy. For crosslinked gelatin, irradiation of the e-beam was performed in air at room temperature. The doses were 100, 200, 300, 400, 500, and 600 kGy. For each treatment, the accelerating voltage of the e-beam energy and current were 1 MeV and 17 mA, respectively, and the dose rate of the e-beam was 8.33 kGy/s.
Scanning electron microscopy
The surface morphology of crosslinked and uncrosslinked gelatin samples was observed using a scanning electron microscope (SEM; JSM-6380; JEOL, Japan). Crosslinked samples were immersed in purified water and lyophilized to observe the fibrous structure of gelatin. Dry samples of gelatin were observed with 11 kV accelerating voltage after sputter coating with platinum. The diameters of nanofiber strands were determined using an image measurement software (I-solution Lite, IMT i-solution Inc., Korea).
Pore size and porosity
The pore size and porosity of the gelatin nanofiber sheets were determined by multiple point Brunauer, Emmet and Teller (BET) gas adsorption measurement using NOVA 2000 and Autosorb-1-C instruments (Quantachrome, Japan).
Measurement of molecular weight
Changes in the molecular weight of each e-beam-irradiated uncrosslinked gelatin sheet were determined using gel permeation chromatography (GPC; Breeze System, Waters, USA) at 40 °C with a refractive index detector. We used 0.02 N NaNO3 as a solvent with a flow rate of 0.8 mL/min. The GPC calibration curve was obtained using pullulan standards.
Quantification of crosslinking degree
where the subscripts c and u stand for the crosslinked and uncrosslinked gelatin, respectively (n = 3).
Nonenzymatic biodegradation test
where W i is the initial weight of the gelatin sheet, and W f is the weight of the gelatin sheet after the degradation test (n = 5).
Water absorption test
The hydrophilicity of the e-beam irradiated gelatin sheets was evaluated using a contact angle analyzer (Phoenix 300; SEO Co., Ltd., Korea) by measuring the complete water absorption time from a deposited droplet of purified water onto the surface of the irradiated gelatin nanofiber sheets at 25 °C and 50% humidity. The results were expressed as the mean ± standard deviation (n = 5).
Fibroblasts (NIH-3 T3 cells) were used to evaluate cell proliferation on e-beam-irradiated gelatin nanofiber scaffolds. Samples were cut into a disk shape (22 mm in diameter), immersed in 70% ethanol for sterilization for 24 h, and then rinsed with PBS for 24 h before seeding. Prepared gelatin fibrous sheets were placed in 12-well culture plates with glass rings to prevent floating. Cells were seeded at a density of 5.0 × 104 cells/disk in 1 mL Dulbecco’s modified Eagle medium (DMEM; Welgene, Korea) containing 10% fetal bovine serum (FBS; Welgene, Korea) and 1% antibiotics (Penicillin-Streptomycin solution; Welgene). Seeded cells were cultured for 1, 3, 5, or 7 days under standard cell culture conditions. After the designated culture period, the culture medium was replaced with 1 mL of medium containing 10% WST-1 reagent. Subsequently, samples were incubated under standard cell culture conditions for 2 h, and 100 μL of the incubated solution was then transferred to a 96-well culture plate. A microplate reader (PHOmo; Autobio Labtec Instruments Co., Ltd., China) was used to measure the absorbance of formazan at 450 nm.
Nonirradiated and irradiated (200 kGy) crosslinked gelatin scaffolds were used for tissue culture experiments at a density of 5.0 × 105 cells/cm2 with 15 mL cell culture medium. Cell-seeded gelatin scaffolds were rinsed with medium to eliminate detached cells and incubated for 3 weeks in a CO2 incubator, with daily changes in culture medium. After incubation, the tissue-scaffold constructs were fixed in 4% formaldehyde aqueous solution and processed for routine paraffin embedding and sectioning. The cell cultured gelatin scaffold sections were stained with hematoxylin and eosin (H&E) to evaluate migration into the gelatin sheet and observed under an optical microscope (Eclipse TS100; Nikon, Japan) equipped with a digital camera (DS-Fi-2; Nikon, Japan).
Values are expressed as means ± standard deviations. Statistical analysis was performed using Student’s t-tests. Results with p values of less than 0.05 were considered significant.
Morphologies and molecular weights of uncrosslinked gelatin nanofibers
Morphology of crosslinked gelatin nanofibers
Structural properties of fibrous gelatin sheets after crosslinking with glutaraldehyde vapor (n = 50)
Fiber diameter (nm)
Pore size (μm)
Uncrosslinked gelatin sheet
443 ± 101
Crosslinked gelatin sheet
2069 ± 865
Crosslinking degree of gelatin nanofibers
The degree of crosslinking after electron beam irradiation with varied irradiation doses (100, 200, 300, 400, 500, 600 kGy) was, 40 ± 3, 37 ± 3, 35 ± 2, 27 ± 4, 22 ± 5, 16 ± 4%. The degree of crosslinking in nonirradiated crosslinked gelatin was 48 ± 4% and decreased as e-beam irradiation increased, reaching a minimum value of 15.5%. The results indicated that the high energy of e-beams promoted the cleavage of the chemical bonds of gelatin, including the site of crosslinking. However, the morphologies of crosslinked gelatin nanofibers after e-beam irradiation were not significantly different from those of nonirradiated crosslinked gelatin (Fig. 3b–g).
Hydrophilicity of e-beam-irradiated gelatin nanofiber sheets
Cell proliferation on e-beam-irradiated gelatin scaffolds
In this study, we focused on not only nanofibrous morphology of gelatin sheet scaffolds but also degradation of gelatin molecules. For instance, we investigated optimum e-beam radiation for molecular degradation as a gelatin nanofiber sheet scaffold. Electrospun gelatin fibrous sheets treated with e-beam irradiation maintained fibrous networks without morphological deformation for both uncrosslinked and crosslinked gelatin (Figs. 1 and 3). E-beam irradiation could modify polymeric properties by changing the structures of macromolecular chains without microstructural deformation. In the radiation chemical reaction, crosslinking and degradation rate compete with each other, and predominance is determined by the molecular structure, presence of additives (such as initiators and crosslinking agents), and radiation kinetic conditions (such as moisture, temperature, pressure, and radiation conditions). Irradiation of polypeptide-based materials in the solid state generally leads to polymeric chain scission rather than crosslinking because polypeptide structures include many intermolecular forces. However, the molecular weights of gelatin nanofibers irradiated in an N2 atmosphere are increased at under 60 kGy (Fig. 2). This result can be explained by the formation of intermolecular networks between gelatin molecules by high-energy e-beams, similar to other crosslinking methods, and these conditions can be used for crosslinking of gelatin materials. However, the modified gelatin nanofibers were dissolved in water (data are not shown), and increases in molecular weight were not sufficient for producing sufficiently modified biomaterials.
Crosslinked gelatin nanofibers enabled modification of the polymeric molecular chain without microstructural deformation by irradiation with e-beams. The degree of crosslinking is mainly correlated with the lifespan of the biomaterials, and highly crosslinked biomaterials can resist both enzymatic degradation and hydrolysis because the degradation rate is generally related to molecular weight and crosslinking density. Accordingly, e-beam irradiation could be an effective method for adjustment of degradation rates in vitro and in vivo. Notably, amide bonds are more resistant to hydrolysis than ester bonds, and biodegradation of crosslinked proteins rarely occurs in vitro since in vitro conditions are different from the conditions observed in vivo. For this reason, scaffolds made of crosslinked proteins can be implanted into animals or can use enzymes for degradation.
In crosslinked gelatin, high irradiation dosages decreased the crosslinking density and affected the biodegradation (Figs. 4 and 5) and hydrophilicity (Fig. 6) of gelatin. Higher irradiation doses applied to crosslinked sheets caused more cleavage of crosslinked gelatin. After irradiation at over 400 kGy, the weight after 1 week was dramatically decreased, and weight loss at 2, 3, and 4 weeks was insignificant. This phenomenon could be responsible for the weight loss of crosslinked sheets through release of short gelatin chains formed after cleavage of chemical bonds by high dosages of e-beam irradiation and exposure to remaining free radicals generated after e-beam treatment.
Changes in water absorption rates were correlated with crosslinking and irradiation. In collagenous materials, previous studies showed that the water absorption ability decreased after crosslinking because the reaction between the ε-amino group and functional group in a crosslinking agent could weaken protonation. As mentioned above, polymeric chain scission and decreased crosslinking after e-beam irradiation could cause increased water absorption ability. Another reason is the direct correlation with e-beam irradiation. After e-beam treatment, the polar component and surface tension of gelatin increased, and this enhancement was related to the decrease in surface hydrophobicity because of reorganization of hydrophilic groups or generation of charged groups on the surface.
The scaffold should keep their physical and chemical structure before cell attachment and proliferation. Then, the scaffolds are degraded according to meet tissue formation. The immediate effect of e-beam irradiation and increased hydrophilicity after e-beam treatment on cell attachment and proliferation were not observed (Fig. 7). However, cultured fibroblasts on gelatin sheets irradiated at 100 and 200 kGy could migrate into sheets and proliferate on both the surface and inner part of the crosslinked gelatin. The structural collapse of gelatin sheets irradiated at more than 300 kGy was determined via microstructural analysis; cells could not migrate into the inner part of the material and proliferated only on the surface. Moreover, noncrosslinked gelatin did not allow proliferation in the inner part compared with irradiated gelatin because the degree of swelling of crosslinked collagenous materials decreased as the crosslinking density increased. Furthermore, irradiated gelatin was easily degraded in PBS.
Migration of proliferated cells into a scaffold is essential for cultivation of soft tissues. To facilitate migration of fibroblasts into the gelatin nanofiber scaffolds, biodegradation should be induced in a week to ensure the inner space of proliferated cells and transportation of nutrients, oxygen and wastes. The gelatin nanofiber scaffold treated with 300 kGy e-beam irradiation showed tissue migration compared to the control scaffold. Based on our SEM, weight loss, cell proliferation and tissue formation results, the 300 kGy e-beam radiation dose demonstrated appropriate condition for soft tissue engineering application.
Electrospun gelatin fibrous sheets treated with e-beam irradiation maintained fibrous networks without morphological deformation for both uncrosslinked and crosslinked gelatin. The molecular weight data of uncrosslinked gelatin as a function of e-beam irradiation revealed that gelatin nanofibers irradiated at under 60 kGy in an N2 atmosphere were crosslinked by high-energy e-beam irradiation. In crosslinked gelatin, high irradiation dosages decreased the crosslinking density and affected the biodegradation and hydrophilicity of gelatin. Physicochemical properties were altered by e-beam irradiation, but the immediate effects of e-beam irradiation on cell attachment and proliferation were not observed. E-beam irradiation could modify the properties of both of uncrosslinked and crosslinked gelatin nanofibrous sheets by changing macromolecular chains without microstructural deformation. In particular, irradiation of crosslinked gelatin resulted in biodegradation without enzyme in PBS, and the lifespan of crosslinked gelatin could be modulated by adjusting the irradiation dosage, demonstrating its potential applications in tissue engineering.
This research was supported by the Human Resource Training Program for Regional Innovation and Creativity funded by the Ministry of Education and National Research Foundation [NRF-2014H1C1A1066917]; the Basic Science Research Program [2015M2A2A6A03044942]; and Research Program to Solve Social Issues [2015M3A9D7067457] of NRF funded by the Ministry of Science, ICT & Future Planning.
Availability of data and materials
The research was designed and coordinated by OHK. The scaffold fabrication and analysis was performed by JBL. The research direction, specific analysis and writing were supported by YGK. WHP and DC revised and improved the final manuscript. All authors read and approved the final manuscript.
Ethics approval and consent to participate
Consent for publication
The authors declare that there are no competing interests regarding the publication of this paper.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The Creative Commons Public Domain Dedication waiver (http://creativecommons.org/publicdomain/zero/1.0/) applies to the data made available in this article, unless otherwise stated.
- Ulubayran K, Ebruaksu S, Gurhan ID, Serbetci K, Hasirci N. Cytotoxicity evaluation of gelatin sponges prepared with different crosslinking agents. J Biomater Sci Polym Ed. 2002;13:1203–19.View ArticleGoogle Scholar
- Zhang S, Huang Y, Yang X, Mei F, Ma Q, Chen G, et al. Gelatin nanofibrous membrane fabricated by electrospinning of aqueous gelatin solution for guided tissue regeneration. J Biomed Mater Res A. 2009;90A:671–9.View ArticleGoogle Scholar
- Chandrasekaran AR, Venugopal J, Sundarrajan S, Ramakrishna S. Fabrication of a nanofibrous scaffold with improved bioactivity for culture of human dermal fibroblasts for skin regeneration. Biomed Mater. 2001;6:1–10.Google Scholar
- Lien SM, Li WT, Huang TJ. Genipin-crosslinked gelatin scaffolds for articular cartilage tissue engineering with a novel crosslinking method. Mater Sci Eng C. 2008;28:36–43.View ArticleGoogle Scholar
- Bigi A, Cojazzi G, Panzavolta S, Rubini K, Roveri N. Mechanical and thermal properties of gelatin films at different degrees of glutaraldehyde crosslinking. Biomaterials. 2001;22:763–8.View ArticleGoogle Scholar
- Zhang YZ, Venugopal J, Huang ZM, Lim CT, Ramakrishna S. Crosslinking of the electospun gelatin nanofibers. Polymer. 2006;47:2911–7.View ArticleGoogle Scholar
- Li JK, Wang N, Wu XS. Gelatin nanoencapsulation of protein/peptide drugs using an emulsifier-free emulsion method. J Microencapsul. 1998;15:163–72.View ArticleGoogle Scholar
- Digenis GA, Gold TB, Shah VP. Cross-linking of gelatin capsules and its relevance to their in vitro- in vivo performance. J Pharm Sci. 1994;8:915–21.View ArticleGoogle Scholar
- Choi YS, Hong SR, Lee YM, Song KW, Park MH, Nam YS. Study on gelatin-containing artificial skin: I. Preparation and characteristics of novel gelatin-alginate sponge. Biomaterials. 1998;20:409–17.View ArticleGoogle Scholar
- Bigi A, Cojazzi G, Panzavolta S, Roveri N, Rubini K. Stabilization of gelatin films by crosslinking with genipin. Biomaterials. 2002;23:4827–32.View ArticleGoogle Scholar
- Ratanavaraporn J, Rangkupan R, Jeeratawatchai H, Kanokpanont S, Damrongsakkul S. Influences of physical and chemical crosslinking techniques on electrospun type a and B gelatin fiber mats. Int J Biol Macromol. 2010;47:431–8.View ArticleGoogle Scholar
- Bhat R, Karim AA. Ultraviolet irradiation improves gel strength of fish gelatin. Food Chem. 2009;113:1160–4.View ArticleGoogle Scholar
- Leontiou I, Matthopoulos DP, Tzphlidou M, Glaros D. The effect of gamma irradiation on collagen fibril structure. Micron. 1993;24:13–6.View ArticleGoogle Scholar
- Woods RJ, Pikaev AK. Applied radiation chemistry: radiation processing. New York: Wiley-Interscience Publication; 1994.Google Scholar
- Kausch H. Radiation effects on polymers for biological use. Berlin: Springer; 1991.Google Scholar
- Benbettaïeb N, Karbowiak T, Brachais C-H, Debeaufort F. Impact of electron beam irradiation on fish gelatin film properties. Food Chem. 2016;195:11–8.View ArticleGoogle Scholar
- BenBettaïeb N, Karbowiak T, Bornaz S, Debeaufort F. Spectroscopic analyses of the influence of electron beam irradiation doses on mechanical, transport properties and microstructure of chitosan-fish gelatin blend films. Food Hydrocoll. 2015;46:37–51.View ArticleGoogle Scholar
- Scott G. Mechanisms of polymer degradation and stabilization. Netherlands: Springer; 1990. p. 109–33.Google Scholar
- Gilbert DL, Kim SW. Macromolecular release from collagen monolithic devices. J Biomed Mater Res A. 1990;24:1221–39.View ArticleGoogle Scholar
- Jiang B, Wu Z, Zhao H, Tang F, Lu J, Wei Q, et al. Electron beam irradiation modification of collagen membrane. Biomaterials. 2006;27:15–23.View ArticleGoogle Scholar
- Powell HM, Boyce ST. Fiber density of electrospun gelatin scaffolds regulates morphogenesis of dermal-epidermal skin substitutes. J Biomed Mater Res A. 2008;84A:1078–86.View ArticleGoogle Scholar
- Choi YS, Hong SR, Lee YM, Song KW, Park MH, Nam YS. Studies on gelatin-containing artificial: II. Preparation and characterization of cross-linked gelatin-hyaluronate sponge. J Biomed Mater Res A. 1999;48:631–9.View ArticleGoogle Scholar